Pergnmon
SolidSto!cElecrronirsVol. 40. Nos l8, pp. 85118.1996 Copyrightcil 1996ElsevierScienceLtd Printedin Circa1 Britain. All rights resewed 003&1101(95)002189 00381101/96 515.00+0.00
MODULATION OF FAN0 RESONANCES BY AN EXTERNAL MAGNETIC FIELD IN SEMICONDUCTOR QUANTUM WELLS V. BELLANI’t,
E. PkREZ’, S. ZIMMERMANN’.
L. VIaA’,
R. HEY2 and K. PLOOG’
‘Departamento de Fisica de Materiales. CIV, Universidad Auton6ma. Cantoblanco, E28049 Madrid, Spain ‘Paul Drude lnstitut fiir Festkiirperelektronik. Hausvogteiplatz 5, D101 I7 Berlin, Germany AbstractWe have studied the dimensionality dependence of the behavior of Fano resonances in the photoluminescence excitation spectra of GaAsAI,Ga, _,As heterostructures in a magnetic field applied in the Faraday configuration. A striking difference is observed between quasitwo and quasithreedimensional systems: while the Fano profiles evolve into Lorentzian lineshapes in twodimensional systems, Fano resonancesemerge from the continuum in threedimensionalsystems with increasing magnetic field.
A Fano resonance in optical spectra is characterized by the asymmetric lineshape resulting from the interference of a discrete state and an energetically degenerate continuum of states[ I]. Fano resonances are generally observed in atomic physics, for instance in the absorption spectra of raregases due to interactions between autoionization thresholds. In semiconductor physics this phenomenon has been reported mostly in the Ramanscattering spectra of doped semiconductors[f]. Although the existence of Fano resonances in the interband optical absorption of quantum wells (QW’s) was predicted in the past [3,4], there is, to the best of our knowledge, only one experimental report in the literature[S]. More recently, a clear observation of Fano resonances in the absorption spectra of highquality bulk GaAs was made by Glutsch et 01.[6]. In their work they demonstrate that the coupling between the discrete states and the continuum is due to the Coulomb interaction. Previously, Becker et a[.[71 reported on magnetoabsorption spectra of GaAs, which displayed sharp, asymmetric lineshapes; however. they did not assign these structures to Fano resonances. In this work we study the evolution of Fano resonances in “quasibulk” GaAs and GaAsAl,Ga, _ ,As QW’s in the presence of an external magnetic field by means of lowtemperature photoluminescence excitation (PLE) spectroscopy. The samples were grown by molecular beam epitaxy on semiinsulating GaAs substrates. The “quasibulk” sample consists of a 200nm GaAs buffer followed by SOOnm of AlO_,Ga,,eAs, a 500nm GaAs layer and 300nm Al,,,Ga,,,As. The structure is capped by a IOnm tPennanent address: Dipartimento di Fisica “A. Volta”, Via Bassi 6, I27100 Pavia, Italy. $In all the following we design the light polarization in the system of reference of the laboratory.
thick GaAs top layer. In the QW sample a 200nm GaAs buffer layer is followed by 20 periods of GaAsAlAs QW’s (5nm well and barrier width), a 1%nm GaAs layer, a 15nm Al,,JGao.,As layer and 10 GaAs QW’s (20nm wide) separated by 97.5nm Al,,G~,,As barriers. This sample is capped by a 3nm GaAs layer. PLE spectra were recorded at 2 K with the magnetic field, up to 13 T, applied in the growth direction z (Faraday configuration). The photoluminescence was excited with light from a Tisapphire laser pumped by an Ar+ion laser. Right handed, u +, and left handed, g, circular polarization of the exciting beam was achieved with an achromatic 114 plate.1 Figure I compiles the PLE spectra of the SOOnm quasibulk GaAs for different magnetic fields and a +polarization of the exciting light. The two lowestlying peaks in the spectra correspond to the heavyhole and lighthole ground state excitonic transitions. The degeneration at the top of the valence band of GaAs is lifted by a small strain present in the sample [8]. which yields a splitting of * 1 meV. The very high quality of the sample is revealed by the observation of the n = 2 and n = 3 excited states of the heavyhole exciton, which are clearly seen close to I .52 eV in the zero field spectrum. In this spectrum we also observe that the PLEintensity decreases with increasing energy. This dependence of the PLEintensity contrasts with the one obtained in the absorption spectra. which reproduces the joint density of states[6]. In fact, PLE measures a pseudoabsorption, which is affected by radiative and nonradiative recombination processes. In contrast to quasitwodimensional semiconductors, where the PLE mimics the shape of the absorption spectra, the luminescence intensity in bulk crystals decreases with increasing excitation energies, due to a higher probability of scattering events leading to nonradiative recombination. In the presence
V. Bellani ef al.
3T I .?S T 0.75 T 0.5 T 0.25 T OT L.
I.S,
I.52
1.54
I .56
I .58
I 60
Energy (eV)
Fig. 1. Lowtemperature (2 K) PLE spectra of quasibulk GaAs for different magnetic fields under u + circularly polarized excitation. The dashed lines are guides to the eye and show the energy shift of the heavyhole magnetoexcitonic transitions with the field.
of a magnetic field the PLE spectra changes dramatically: asymmetric resonance features appear, and become stronger and blueshifted with increasing field. Moreover, the decrease in the continuum pseudoabsorption, which was observed at zero field, gradually disappears with increasing field and the PLE spectra becomes similar to absorption spectra (see below). The lineshape of these resonances can be interpreted as Fano resonances[l] arising from the interference of magnetoexcitons and the continua of lower lying Landau levels. The theory of excitonic states of semiconductors in magnetic field was treated extensively by Altarelli and Lipari]9]. For each pair of conduction and valenceband Landau levels. with the same Landau quantum number N,,, there are associated magnetoexcitonic transitions which give rise to the most prominent features of the absorption spectra. The presence of a magnetic field does not affect the wave vectors along the direction of the field. and therefore for each Landau level a onedimensional continuum prevails. Two different series of Fano resonances are readily identified in the spectra of Fig. 1. Those with lower oscillator strength. as for example the one labeled N, (Ih). correspond to resonances arising from lighthole magnetoexcitons, while the resonances with larger oscillator strength, e.g. N,(hh), are due to heavyhole magnetoexcitons. The two energetically lowest light and heavyhole magnetoexcitons (N,) and their excited states lie below the continuum and consequently do not show interferences. Their lineshapes are Lorentzian for all magnetic fields. The energy degeneration of the higher
tWc will use the following notation to label the transitions: h(l) means heavy (light) hole; a subindex indicates the same confined subband for electrons and holes; in the case of two subindicesthe former correspondsto electrons and the latter to holes. The notation in the parentheses corresponds to the labeling of hydrogeniclike states.
(
I
I s3
1.54
I
I
ss
I
I Sh
I
I.9
Energy (eV) Fig. 2. Lowtemperature PLE spectra of a 200kl GaAsAl,,,Gq,,As QW for different magnetic fields under C+ circularly polarized excitation. Down and up arrows point to the h,,(l s) and h,(l s) excitonic transitions, respectiveJy. The dotted lines help to observe the evolution from Fano profiles at zero field to Lorentzianlike lineshapes at higher fields.
order magnetoexcitonic transitions, e.g. N, , with the onedimensional continua of lower lying Landau levels results in asymmetric lineshapes associated with Fano resonances. The behavior of the magnetoexcitons in a quasitwo dimensional structure is markedly different to that observed in the quasithreedimensional sample. Figure 2 shows PLE spectra of the 200A QW for different magnetic fields and u + exciting light. For a QW, the confinement of the carriers gives rise to a closer resemblance between the PLE and the optical absorption. At all fields, the spectra presents excitonic structures lying on a continuum which flattens and decreases with increasing field. The first peak in the spectra corresponds to the ground state of the lighthole exciton I,( 1 s)t and has a FWHM of 0.5 meV. The narrowness of the peaks and the absence of Stokes shift between h,( I s) in emission and PLE spectra. which prevents the observation of the heavyhole exciton in PLE, reveals the very high quality of our sample. This is also manifested by the observation at zero field of the first excited states of the h, and I, excitons. In the zero field spectrum two asymmetric structures, which are assigned to the /I,,( I s) and h,( I s) transitions[ IO], are clearly observed. These discrete excitonic states interfere with the continua of lower lying energy levels, giving rise to Fano resonance lineshapes. increasing the field, new structures which correspond to excited states of magnetoexcitons appear. Moreover, the Fano resonances progressively lose their asymmetric shape and become more Lorentzianlike, resembling closer a pure excitonic transition, like the first excited state of the hhexciton, labeled h, (2 s) in the spectra at 3 T. This is due to the splitting of the twodimensional continuum, with increasing field, into discrete levels, which leads to a suppression of the interference paths and causes the disappearance of the Fano profiles. Concurrently, the background of the spectra diminishes, because
81
Modulation of Fano resonances by an external magnetic field the application of the magnetic field in the Faraday configuration effectively reduces the dimensionahty of the system to zero. In a zerodimensional semiconductor the joint density of states is zero at all energies, except at those corresponding to magnetoexcitonic transitions. In a similar way, the application of a magnetic field to a bulk semiconductor decreases the dimensionality of the system to one, therefore reducing the efficiency of nonradiative recombination processes. This explains why in the quasithree dimensional sample the PLE and the absorption spectra become similar at high fields. We fitted the experimental Fano resonance lineshapes with the expression[l I]
Energy (eV) 1.538 1.540
B=
200 QW
with t a reduced energy given by
where El is the energy of the discrete transition and F is the transition rate between the ground state and the continuum
r=?p h V is the coupling matrix element. The parameter q characterizes the ratio between the coupling of the ground state to the discrete state and of the former to the continuum. In particular, its squared magnitude is proportional to the relative oscillator strength of the magnetoexciton compared to that of the continuum states. Its sign depends on the relative signs of the matrix elements of the transition amplitudes to the discrete state, to the continuum and of the coupling matrix element between the discrete state and the continuum. This sign determines whether the maximum or minimum of the lineshape occurs on the lowenergy side of the line. q > 0 corresponds to a lineshape where the minimum of the Fano profile lies at smaller energies than the maximum, while q < 0 corresponds to the opposite situation. Figure 3 presents two experimental Fano profiles for the QW (open circles, upper scale) and the quasithree dimensional sample (black squares, lower scale), together with the fits to eqn (1) (lines). For the QW the Fano resonance corresponds to the h,,(l s) magnetoexciton at 0.5 T, and the fit gives q = 2.1. A fit of the Fano resonance lying at 1.556 eV (h,(l s) in Fig. 2) obtains a q of  3.1. At 3 T, the fits of the lineshapes yield values of q of 14.7 and  10.5 for h,,(l s) and h,(l s), respectively. This demonstrates the disappearance of the Fano resonances at higher magnetic fields, because the higher absolute values of q indicate more Lorentzianlike lineshapes (q + f 00 for an ideal Lorentzian). The opposite sign of q for the two magnetoexcitons means that there is a change in one or more of the signs of the matrix elements on which q depends. Indeed, the larger absolute value
Is50
1.552
I.554
I .556
Energy (eV) Fig. 3. Experimental Fano profiles and their corresponding fits to eqn (1). Open circles (upper scale) show the experimental Fano resonance associated with the h,,(l s) transition at OST for the QW sample (dashed line, fit). Full squares (lower scale) present the experimental N, (hh) Fano structure at IOT in the quasibulk sample (continuous line. fit).
of q for the h2( 1 s) transition, as compared with that of the hu(l s), denotes that the presence of the continuum of states affects more efficiently the latter exciton than the former one, and that the Fano asymmetry is more pronounced. For the 500nm GaAs sample the value of q is negative for all Fano structures. As an example, we show the Fano resonance corresponding to N,(hh) for a field of 10T in Fig. 3 together with its fit to eqn (I), which obtains a value of q of 2.9. The accuracy of the fits and the evolution of the lineshapes with magnetic field confirm the correct interpretation of the structures as Fano resonances. Many different mechanisms could be responsible for the coupling between the discrete state and the continuum, giving rise to Fano resonances. Due to the coulombic nature of the magnetoexcitons, and based on recent calculations[6], which demonstrate that the nondiagonal Coulomb interaction between the magnetoexcitons and the continua can provide the coupling for the interferences, we believe that the Coulomb interaction is the most plausible candidate to produce the appearance of Fano profiles in the PLE spectra of semiconductor heterostructures. The assignment of the asymmetric peaks observed in Fig. 1 to Fano resonances is also established by the dependence of their energies on the magnetic field, which is compiled in Fig. 4. The experimental points are obtained from a complete lineshape analysis
88
V. Bellani et al.
Ihu
N,(hh)

a+excilation 1.5x 
,
, _
N,(hhi” n’
4
T=2K A
/‘ 9’
5
2! 22 1.56 k2
A 4
.’ c’
N,(hh) .’ J d
5 1.54
structures in the presence of a magnetic field. The evolution of the resonances with the field is markedly different in the two cases. In threedimensional semiconductors, Fano resonances appear and become stronger with increasing field, whereas in twodimensional semiconductors they are clearly resolved at zero field, and progressively evolve into Lorentzian peaks for higher magnetic fields. A complete lineshape analysis of the resonances allows us to obtain the parameters of the Fano profiles and their evolution with the magnetic field. wish to thank C. Tejedor for fruitful discussions. This work was partially supported by the Spanish CICyT Grant no. MAT940982X02 and by “European HC Mobility” Program MagNET CHRXCT920062. V.B. and S.Z. want to thank the Fondazione Francesco Somaini and the Dr Carl Duisberg Stiftung, respectively, for financial support. AcknowledgementsWe
I.52 
Fig. 4. Energies of three heavyhole Fano resonances corresponding to the Landau levels N = 1,2,3 as a function of the magnetic field under u + circularly polarized excitation for the 500nm GaAs sample. The lines are best fits to a linear dependence, which is valid at high fields (see text).
REFERENCES
1. U. Fano, Phys. Rev. 124, 1866 (1961). 2. See, e.g., Light Scattering in Solids IV (Edited by M.
Cardona and G. Giintherodt), of the resonances according to eqn (1). At higher fields (B > 2 T), the energies of the three structures (N,(hh), N2(hh), and N,(hh)) vary linearly with field, in agreement with the expected dependence of the ground states of the magnetoexcitons associated to the different Landau transitions (at lower fields the dependence is quadratic). From an analysis of the fancharts it is also possible to confirm the light or heavyhole character of the resonances[6]. The energies at which magnetoexcitonic transitions occur do not follow exactly the dependence for Landau levels, (n + 1/2)ho,, because of their excitonic character and the fact that the binding energy decreases for increasing N,. In summary, we have presented the distinct behavior of Fano resonances in the PLE spectra of quasithreeand quasitwo dimensional GaAsAl, Ga , _i As hetero
Topics
in
Applied
Vol. 54. Springer, Berlin (1984). 3. D. A. Broido and L. J. Sham, Phys. Re~j. B 34, 3917 (1986). 4. H. Chu and Y.C. Chang, Whys.Rev. E 39,10861(1989). 5. D. Y. Oberli, G. &hm, G. Weimann and J. A. Brum, Phys. Ray. B 49, 5757 (1994). 6. S. Glutsch, U. Siegner, M. A. Mycek and D. S. Chemla, Phys. Rev. i9 So, 17009 (1994). 7. W. Becker, B. Gerlach, T. Homung and G. Ulbrich, in Proceedings of the 18th International Conference on the Physics of Semiconductors (Edited by 0. Engstrom), p. 1713. World Scientific, Singapore (1987). 8. F. H. Pollack and M. Cardona, Phys. Rev. 172, 816 (1968). 9. M. Altarelli and N. 0. Lipari, Phys. Reu. B 9, 1733 (1974). IO. L. Vitia, G. E. W. Bauer, M. Potemski, J. C. Maan, E. E. Mendez and W. 1. Wang, fhys. Rev. B 41, 10767 (1990). I I. C. CohenTannoudij, J. DupontRot and G. Grynberg. AtomPhoton Interacrions. Wiley, New York (1992). Physics,